MICROSTRUCTURE, MECHANICAL PROPERTIES AND SLIDING W 2020-01-02¢ Microstructure,...
Embed Size (px)
Transcript of MICROSTRUCTURE, MECHANICAL PROPERTIES AND SLIDING W 2020-01-02¢ Microstructure,...
www.tjprc.org SCOPUS Indexed Journal firstname.lastname@example.org
MICROSTRUCTURE, MECHANICAL PROPERTIES AND SLIDING W EAR
BEHAVIOUR OF SILICON CARBIDE REINFORCED AL 6026 COM POSITES
H. M. SOMASHEKAR 1, GOWTHAMA. K 2 & B. SURESHA3
1,2Department of Mechanical Engineering, Dr. Ambedkar Institute of Technology, Bengaluru, Karnataka, India
3Department of Mechanical Engineering, The National Institute of Engineering, Mysuru, India
In this research work, the role of fine silicon carbide (SiC) particles on mechanical properties and dry sliding wear
behaviour of Al 6026 composites were investigated. Al 6026 matrix reinforced with different weight percentages (3, 5, 7,
and 10) of SiC particles have been fabricated following liquid metallurgy route. Microstructure, hardness, and tensile
properties of these composites were evaluated and compared with Al 6026. In addition, dry sliding wear behaviour of Al
6026 based composites were conducted using pin-on-plate wear test rig. Worn-out coupons of the selected composites
were analyzed using scanning electron microscope for predicting the involved wear mechanisms. The major findings
are: i) Al 6026 composites showed improved hardness, tensile strength and Young’s modulus, ii) tensile properties of Al
6026/10% SiC composites were lower than Al 6026/7% SiC indicating that the critical weight fraction of SiC in Al 6026
is 7%, iii) specific wear rate of Al 6026 and SiC reinforced Al 2026 composites increases with increasing applied normal
load and coefficient of friction decreases slightly at higher load, and iv) specific wear rate and friction coefficient of Al–
SiC are lower than that of unreinforced Al 6026. These results reveals the effect of SiC reinforcement on improved
mechanical properties, reduced friction coefficient, and better wear resistance of Al 6026 composites and provide a
useful attendant for healthier control of their wear.
KEYWORDS: Al 6026/SiC Composites, Microstructure, Tensile Properties, Wear & Worn Surface Topography
Received: Oct 15, 2019; Accepted: Nov 05, 2019; Published: Jan 02, 2020; Paper Id.: IJMPERDFEB202022
Metal matrix composites (MMCs), are principally metallic alloys strengthened with characteristically ceramic
particulates. The most common matrix alloys engaged are aluminium (Al), magnesium and titanium. Al is the
furthermost exploited metal alloy as matrix in the growth of Al based composites and the elucidations for this have
been described [1, 2]. The ultimate properties of Al based composites governed by the inherent properties of
reinforcement selected and the type of Al alloy. Moreover, the processing method tailed for manufacturing of Al
based composites also influence the final properties. This is because, most of the parameters put into deliberation
during the design of Al based composites are allied with the ceramic particulates. Major parameter includes
reinforcement type, size, shape, modulus of elasticity, hardness, distribution and interface between the
reinforcement and matrix .
Aluminium amid some numerous metals is attractive due to its anticipated properties such as ductility,
malleability, good conductivity, lightweight, functional strength and availability in abundance (8% of earth crust is
Al). In conglomeration with sturdy materials like ceramic such as SiC, B4C, TiC, etc. are used to develop
composites. The improved properties of the composites lead to finding a wide range of applications in industries
O riginal A
rticle International Journal of Mechanical and Production Engineering Research and Development (IJMPERD) ISSN(P): 2249–6890; ISSN(E): 2249–8001 Vol. 10, Issue 1, Feb 2020, 259–270 © TJPRC Pvt. Ltd.
260 H. M. Somashekar, Gowthama. K & B. Suresha
Impact Factor (JCC): 8.8746 SCOPUS Indexed Journal NAAS Rating: 3.11
and structural applications (aerospace, automotive, marine, and military) [3–6].
The information on usage of ceramics are very limited, for instance, Laksmikanathan et al.  studied the addition
of SiC (dual size) in Al-MMCs and showed an improvement in mechanical and wear resistance of the composites.
Hayrettin et al.  studied the additions of combination of ceramics namely Al2O3 and SiC (hybrid MMCs) in Al matrix
and demonstrated improved hardness, compression strength and wear resistance of the Al matrix alloy. Yadav et al. 
studied the addition of Al-SiC-CNT (multi walled) nano-hybrid composites and indicated an enhancement in mechanical
strength and modulus as well as resistance to wear. Straffelini et al.  concluded that the Al hardness impacts the wear
conduct of Al 6061-Al2O3 composites. How and Baker , in their investigation of wear conduct of Al 6061- saffil
(Al 2O3) fiber and inferred that saffil is noteworthy in enlightening the wear resistance of the composites.
Vanarotti and Co-workers  studied the mechanical properties of SiC reinforced Al 356 composites
manufactured by die-casting process. From the data generated, it was published that the hardness and tensile strength
increased with increase in SiC loading. Though, their work does not provide information about the most optimum
reinforcement in the Al alloy. Muthu Kumar et al.  studied the role of SiC in LM4 alloy processed via stir casting
route. This work showed improvement in wear resistance as well as corrosion resistance. Liang and Co- workers 
concluded that Al based SiC composites display superior wear resistance. Ramesh and Safiulla  contemplated wear of
extruded Al 6061 reinforced with SiC, Al2O3 and cerium oxide fortifications, and presumed that wear rates of extruded Al
6061/cerium oxide had superior wear resistance under similar test conditions. Ramesh et al.  stated that the higher
loading of silicon nitride particles in Al 6061 has brought greater hardness and ultimate tensile strength.
From the above literature review, it is clear that there have been huge research studies on processing and
properties evaluation of SiC and other ceramic particles reinforced MMCs, but an explicit understanding on the effect of
very fine SiC particles (
Microstructure, Mechanical Properties and Sliding Wear Behaviour of Silicon 261 Carbide Reinforced Al 6026 Composites
www.tjprc.org SCOPUS Indexed Journal email@example.com
Table 1: Chemical Composition of Al 6026 Alloy
Element wt. %
Si 1.20 Fe 0.50 Cu 0.25 Mn 0.35 Mg 0.60 Cr 0.10 Zn 0.10 Bi 1.20 Ti 0.10
Others 0.15 Balance 95.45
Fabrication of Composites
The fabrication of Al based composites were carried out by liquid metallurgy route via stir-casting process. Al ingots were
placed in graphite crucible and heated to 800oC in the electrical furnace. Preheated SiC particles were brought into vortex
of the liquid of Al, compounded after viable degassing with degasser namely hexachloroethane tablet. Mechanical stirring
of the liquid metal for duration of 10 min was accomplished by utilizing artistic covered impeller made of steel. Spindle
speed of 400 rpm and a pouring temperature of 800 °C were kept during stir casting process. The liquid metal was filled to
the preheated molds made of cast iron. The cylindrical rods of diameter 30 mm, and length 200 mm cast composites of Al
6026/SiC were achieved. In addition, Al 6026 was also cast for comparison purpose. The designation of the Al matrix and
Al 6026/SiC composites is given in table 2. The cast Al 6026 and Al 6026/SiC composites were machined to prepare the
test coupons as per ASTM standards.
Table 2: Designation of Al 6026 and its Composites Sl. No Composites
(Designation) SiC (~25 µm) wt. %
1 Aluminium(Al 6026) ---- 2 Aluminium + SiC(Al 6026/3SiC) 3 3 Aluminium + SiC(Al 6026/5SiC) 5 4 Aluminium + SiC(Al 6026/7SiC) 7 5 Aluminium + SiC(Al 6026/10SiC) 10
The coupons for microstructure study were prepared as per standard metallurgical procedures (IS: 7739 PART III - 1976
(RA 2007)), etched in etchant prepared using 90 ml water, 4 ml HF, 4 ml H2S04 and 2g Cr03. Carefully polished and mirror
finished coupons were examined under Nikon-Upright metallurgical microscope (Make: Japan, Eclipse Ni-E) as shown in
Figure 1 to obtain micrographs.
Impact Factor (JCC): 8.8746
The hardness tests were accompanied as per ASTM
indenter (diameter of 2.5 mm) and an applied load of 250 kg was used. The duration of load
readings were taken for each coupon, at different positions to circumvent the conceivable effects